3Pitting Corrosion Monitoring Using Acoustic EmissionAcoustic Emission and Advanced Nondestructive Testing Center (ANDT), Department of Production Engineering, Faculty of Engineering, King Mongkuts University of Technology Thonburi, Bangmod, Toong-kru, Bangkok Thailand 1. IntroductionDamage from corrosion represents one of the most important problems in existing structures. Various types of traditional nondestructive testing (NDT) for example, Ultrasonic ThicknessMeasurement (UTM) or Magnetic Flux Leakage (MFL) are implemented to measure the growth of corrosion; each method, however, has its particular limitations. For the last two decades Acoustic Emission (AE), an advanced NDT method, has been used to monitor the severity of corrosion. Compared to the conventional NDT methods, it is less intrusive and has the advantage of real-time measurement. In this chapter, the development of pitting corrosion monitoring using AE is reviewed. AE refers to the generation of transient elastic or stress waves during the rapid release of energy from localized sources within a material. The source of these emissions in metals is closely related to the dislocation movement accompanying plastic deformation and the initiation and extension of cracks in a structure under stress. AE systems are comprised of an AE sensor, an amplifier and filter, an acquisition and a data display. In the corrosion process, an AE parameter is extracted and then the relation with corrosion grading is determined. The parameters commonly used in corrosion applications include AE HIT, Even and AE energy. The accurate forecast of corrosion level assists in maintenance planning. For instance, a storage tank or pipeline in the petroleum industry could fail as a result of pitting. In general, the severity of pitting corrosion is presented with two factors: the maximum pit depth and the pitting factor. A wide variety of methods were used to measure the severity of pitting corrosion. In this chapter, AE sources corresponded to the maximum pit depth are explained. The AE source generated from the pitting corrosion related to its mechanism is exposed. Experimental setup, results and discussions are briefly described. Research works in AE sources are deliberately reviewed. Three AE sources hydrogen bubbles, breakage of passive film and pit growth are proposed. The average frequency of the AE parameter was used to define the hydrogen bubbles. The oscillation, movement, and breakage of hydrogen bubbles generate acoustic stress waves in the same frequency band, which is related to the bubble diameter. An acoustic parameter, namely the duration time, can be used to classify
the AE signal sources generated from the breakage of the passive film into two groups: the rupture of passive films and the pit growth signal. The results were explained based on the corrosion mechanism and the electrochemical analysis. In practice, the location of the pitting can be calculated by using the difference in the arriving time of each pair or group of sensors. In this chapter, a novel source location system using an FPGA-PC system was utilized to calculate the arrival time difference from signals received from an array of three AE sensors on the specimen. The system consists of the AE sensors, pre-amplifiers, a signal conditioning unit, an FPGA module, a PC and a data acquisition. Experimental results and errors are shown.
2. Acoustic Emission testing (AE)Nondestructive Testing can be defined as the development and application of methods to examine materials or components, in ways that do not impair future usefulness and serviceability, in order to detect, locate, measure and evaluate flaws; to assess integrity, properties and composition; and to measure geometric characteristics (American Society for Testing and Materials (ASTM E1316, 2001). Acoustic emission (AE) is a powerful method for non-destructive testing and material evaluation. Older NDT techniques such as radiography, ultrasonic, and eddy current detect geometric discontinuities by beaming some form of energy into the structure under test. AE is different: it detects microscopic movement, not geometric discontinuities. AE, by definition, is a class of phenomena whereby transient stress/displacement waves are generated by the rapid release of energy from localized sources within a material, or the transient waves so generated (ASTM E1316, 2011). AE is the recommended term for general use. Other terms that have been used in AE literature include (1) stress wave emission, (2) microseismic activity, and (3) emission or acoustic emission or emission with other qualifying modifiers. These elastic waves can be detected by microphones or transducers attached to the surface of the specimen. AE techniques have been used in many applications such as in material degradation, leak and flow, solidification, and machining. AE is a passive technique. The growing defect makes its own signal and the signal travels to the detecting sensors. The main benefits of AE compared to other NDT methods are that AE is a real-time method and it is less intrusive. The discontinuities of defects can be detected by AE at an early stage when they are occurring or growing. AE techniques can be used as a warning system before the testing material is severely damaged. AE requires access only at the sensors; while on the other hand, most other NDT techniques require access to all regions inspected. In order to detect AE events, a transducer is required to convert the very small surface displacement to a voltage. Displacements as small as 10-14 metre [(Course Handbook for SNT-TC-1A (1991)] can be detected by the use of the most sensitive sensors. The most common type of transducer is piezoelectric, which is sensitive, easy to apply, and cheap. A couplant is needed for good transmission, and is usually achieved by grease or ultrasonic couplants, together with some means of applying force to maintain contact.
Pitting Corrosion Monitoring Using Acoustic Emission
2.1 AE systems An AE system consists of AE sensor, cable and pre-amplifier, and AE data-acquisition, as illustrated in Figure 1. There are two types of piezoelectric transducer: resonant transducers and broadband transducers. The principal or resonant frequency of a piezoelectric element depends on its thickness. The piezoelectric element is unbacked or undamped in a resonant transducer, but a broadband transducer has an element that is backed with an attenuating medium. The frequencies of most AE-resonant transducers lie in the range of 100 kHz to 1 MHz. However, it was found that the frequency of 30 kHz is often used for corrosion detection. Resonant sensors are more sensitive than broadband types because of the gain provided by mechanical resonance. Broadband sensors are used when the object of interest has the frequency spectrum of AE, but they do not have as high sensitivity as resonant transducers. Because of the reliance on mechanical resonance, resonant sensors can be used to detect preferentially a frequency range which has been shown from previous experience to give a good indication of the AE changes. Alternatively, a broadband sensor can be used and the required frequency is selected by filters.
Fig. 1. Component of AE system (Prateepasen A., 2007) Elastic waves emitted from materials can be divided into 2 types based on their appearance: burst and continuous. A burst emission is a signal, oscillatory in shape, whose oscillations have a rapid increase in amplitude from an initial reference level, generally that of the background noise, followed by a decrease, generally more gradual, to a value close to the initial level. Acoustic emission released from pitting corrosion is of the burst type. A continuous emission is a qualitative term applied to acoustic emission when the bursts or pulses are not discernible. (A pulse is an acoustic emission signal that has a rapid increase in amplitude to its maximum value, followed by an immediate return.) 2.2 AE waveform parameters The parameters commonly used to predict severity in the corrosion process are AE ring down count, AE HIT, AE Even and AE energy or AErms. An AE burst, the typical AE signal from the corrosion process, is shown in Figure 2 and can be described by the parameters as follows.
Duration Peak amplitude Counts=11
Fig. 2. Definition of AE waveform parameters Ring down count is the number of times a signal exceeds a pre-set threshold. This is a simple measure of the signal size, since larger signals typically give more counts. Electronically, this is a very easy measurement, and it was the first to come into widespread use. By summing the counts from all detected emissions, one has a convenient measurement of the total emission from the specimen or structure. The number of counts (N) can be calculated by (Ronnie K.,1987)
N= where B V0Vt
V ln 0 2 B Vt
= angular frequency = decay constant (greater than 0) = initial signal amplitude = threshold voltage of counter
AErms is the root mean squared value of the input signal. Since acoustic emission activity is attributed to the rapid release of energy in a material, the energy content of the acoustic emission signal can be related to this energy release. AErms can be defined asVrms = (1 1 V 2 (t )dt ) 2 T 0 T
= signal voltage function = period of time
AE HIT is the detection and measurement of an AE signal on a channel (ASTM 1316, 2011). AE EVEN is an occurrence of a local material change or mechanical action resulting in acoustic emission.
Pitting Corrosion Monitoring Using Acoustic Emission
AE ENERGY is the energy contained in an acoustic emission signal, which is eval